# Electronic Supplementary Material (ESI) for Chemical Communications.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_bctn
_database_code_depnum_ccdc_archive 'CCDC 1954383'
loop_
_audit_author_name
_audit_author_address
'jinyang li'
;fujian institute of research on the structure
China
;
_audit_update_record             
;
2019-09-18 deposited with the CCDC.	2022-09-08 downloaded from the CCDC.
;
_audit_creation_date             2019-08-30
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         '0.5(Ba2 Co14 Na4 O36 Te6)'
_chemical_formula_sum            'Ba Co7 Na2 O18 Te3'
_chemical_formula_weight         1266.60
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      hexagonal
_space_group_IT_number           176
_space_group_name_H-M_alt        'P 63/m'
_space_group_name_Hall           '-P 6c'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'

_cell_length_a                   9.4283(2)
_cell_length_b                   9.4283(2)
_cell_length_c                   9.0489(2)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     696.62(3)
_cell_formula_units_Z            2.00004
_cell_measurement_reflns_used    6021
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      32.9820
_cell_measurement_theta_min      3.3280
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    17.231
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.48079
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
CrysAlisPro 1.171.39.46 (Rigaku Oxford Diffraction, 2018)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'clear dark violet'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   dark
_exptl_crystal_colour_primary    violet
_exptl_crystal_density_diffrn    6.039
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       needle
_exptl_crystal_F_000             1134
_exptl_crystal_size_max          ?
_exptl_crystal_size_mid          ?
_exptl_crystal_size_min          ?
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0390
_diffrn_reflns_av_unetI/netI     0.0153
_diffrn_reflns_Laue_measured_fraction_full 0.993
_diffrn_reflns_Laue_measured_fraction_max 0.965
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            8212
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.965
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         33.097
_diffrn_reflns_theta_min         2.494
_diffrn_ambient_temperature      293(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.965
_diffrn_measurement_details      
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω   -115.00  65.00   0.50    5.00    --  -25.00  45.00   0.00  360
  2  ω   -115.00  25.00   0.50    5.00    --  -25.00  45.00  90.00  280
  3  ω   -115.00 -35.00   0.50    5.00    --  -25.00  45.00 180.00  160
;
_diffrn_measurement_device       'abstract diffractometer'
_diffrn_measurement_device_type  
'dtrek-CrysAlisPro-abstract goniometer imported rigaku-d*trek images'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type       
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0630010000
_diffrn_orient_matrix_UB_12      -0.0207658000
_diffrn_orient_matrix_UB_13      -0.0527840000
_diffrn_orient_matrix_UB_21      0.0578143000
_diffrn_orient_matrix_UB_22      0.0209360000
_diffrn_orient_matrix_UB_23      -0.0579196000
_diffrn_orient_matrix_UB_31      -0.0153658000
_diffrn_orient_matrix_UB_32      -0.0817173000
_diffrn_orient_matrix_UB_33      -0.0014306000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                843
_reflns_number_total             905
_reflns_odcompleteness_completeness 96.83
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     33.02
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'olex2.refine (Bourhis et al., 2015)'
_computing_structure_solution    'olex2.solve (Bourhis et al., 2015)'
_refine_diff_density_max         1.011
_refine_diff_density_min         -1.830
_refine_diff_density_rms         0.215
_refine_ls_extinction_coef       0.0021(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.178
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     54
_refine_ls_number_reflns         905
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0264
_refine_ls_R_factor_gt           0.0233
_refine_ls_restrained_S_all      1.178
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0128P)²+6.0359P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0505
_refine_ls_wR_factor_ref         0.0514
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     iterative
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Te1 Te 0.35477(3) 0.34359(4) 0.750000 0.00377(9) Uani 1 2 d S T P . .
Co1 Co 0.35846(6) 0.35099(6) 0.40996(5) 0.00630(11) Uani 1 1 d . . . . .
Co2 Co 0.666667 0.333333 0.750000 0.0102(2) Uani 1 6 d S T P . .
Na1 Na 0.333333 0.666667 0.5777(3) 0.0048(4) Uani 1 3 d S T P . .
O3 O 0.4571(4) 0.5803(4) 0.750000 0.0071(6) Uani 1 2 d S T P . .
O2 O 0.2080(3) 0.3168(3) 0.5914(3) 0.0067(4) Uani 1 1 d . . . . .
O4 O 0.5200(3) 0.3862(3) 0.8996(3) 0.0075(4) Uani 1 1 d . . . . .
O1 O 0.2825(5) 0.1120(4) 0.750000 0.0086(6) Uani 1 2 d S T P . .
Ba1 Ba 0.000000 0.000000 0.500000 0.01572(14) Uani 1 6 d S T P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Te1 Co1 3.0776(5) 10_557 ?
Te1 Co1 3.0776(5) . ?
Te1 Co2 2.9902(3) . ?
Te1 Na1 3.5164(11) . ?
Te1 Na1 3.5164(11) 10_557 ?
Te1 O3 1.939(3) . ?
Te1 O2 1.920(2) 10_557 ?
Te1 O2 1.920(2) . ?
Te1 O4 1.948(2) . ?
Te1 O4 1.948(2) 10_557 ?
Te1 O1 1.935(3) . ?
Te1 Ba1 3.9955(2) . ?
Co1 Co1 2.8949(9) 10_556 ?
Co1 Na1 2.9947(5) 7_666 ?
Co1 Na1 3.4532(12) . ?
Co1 O3 2.101(3) 7_666 ?
Co1 O2 2.115(2) 8_556 ?
Co1 O2 2.087(3) . ?
Co1 O4 2.212(3) 10_557 ?
Co1 O4 2.150(3) 4_664 ?
Co1 O1 2.123(3) 9_556 ?
Co1 Ba1 3.4428(5) . ?
Co2 Na1 2.966(2) 4_665 ?
Co2 Na1 2.966(2) 7_666 ?
Co2 O4 2.164(3) 12_667 ?
Co2 O4 2.164(3) 11_657 ?
Co2 O4 2.164(3) 10_557 ?
Co2 O4 2.164(3) 2_655 ?
Co2 O4 2.164(3) . ?
Co2 O4 2.164(3) 3_665 ?
Na1 O3 2.325(3) 2_665 ?
Na1 O3 2.325(3) 3_565 ?
Na1 O3 2.325(3) . ?
Na1 O2 2.898(3) 3_565 ?
Na1 O2 2.898(3) . ?
Na1 O2 2.898(3) 2_665 ?
Na1 O4 2.334(3) 5_564 ?
Na1 O4 2.334(3) 6_554 ?
Na1 O4 2.334(3) 4_664 ?
O2 Ba1 2.756(2) . ?
O1 Ba1 3.243(3) . ?
O1 Ba1 3.243(3) 4 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Co1 Te1 Co1 177.75(2) . 10_557 ?
Co1 Te1 Na1 115.37(4) . 10_557 ?
Co1 Te1 Na1 62.74(4) 10_557 10_557 ?
Co1 Te1 Na1 115.37(4) 10_557 . ?
Co1 Te1 Na1 62.74(4) . . ?
Co1 Te1 Ba1 125.440(12) 10_557 . ?
Co1 Te1 Ba1 56.475(9) . . ?
Co2 Te1 Co1 90.032(10) . . ?
Co2 Te1 Co1 90.032(10) . 10_557 ?
Co2 Te1 Na1 120.758(14) . . ?
Co2 Te1 Na1 120.758(14) . 10_557 ?
Co2 Te1 Ba1 114.325(7) . . ?
Na1 Te1 Na1 52.63(7) . 10_557 ?
Na1 Te1 Ba1 93.67(2) . . ?
Na1 Te1 Ba1 124.467(17) 10_557 . ?
O3 Te1 Co1 88.879(10) . 10_557 ?
O3 Te1 Co1 88.879(10) . . ?
O3 Te1 Co2 96.08(10) . . ?
O3 Te1 Na1 38.17(8) . . ?
O3 Te1 Na1 38.17(8) . 10_557 ?
O3 Te1 O4 82.89(11) . . ?
O3 Te1 O4 82.89(11) . 10_557 ?
O3 Te1 Ba1 131.79(7) . . ?
O2 Te1 Co1 41.86(7) . . ?
O2 Te1 Co1 41.86(7) 10_557 10_557 ?
O2 Te1 Co1 138.53(8) . 10_557 ?
O2 Te1 Co1 138.53(8) 10_557 . ?
O2 Te1 Co2 130.64(7) 10_557 . ?
O2 Te1 Co2 130.64(7) . . ?
O2 Te1 Na1 55.46(8) . . ?
O2 Te1 Na1 55.46(8) 10_557 10_557 ?
O2 Te1 Na1 95.48(8) . 10_557 ?
O2 Te1 Na1 95.48(8) 10_557 . ?
O2 Te1 O3 93.59(10) 10_557 . ?
O2 Te1 O3 93.59(10) . . ?
O2 Te1 O2 96.70(15) . 10_557 ?
O2 Te1 O4 174.67(11) . . ?
O2 Te1 O4 87.54(10) 10_557 . ?
O2 Te1 O4 87.54(10) . 10_557 ?
O2 Te1 O4 174.67(11) 10_557 10_557 ?
O2 Te1 O1 91.58(11) . . ?
O2 Te1 O1 91.58(11) 10_557 . ?
O2 Te1 Ba1 38.21(8) . . ?
O2 Te1 Ba1 93.46(8) 10_557 . ?
O4 Te1 Co1 45.71(8) . 10_557 ?
O4 Te1 Co1 45.71(8) 10_557 . ?
O4 Te1 Co1 133.73(8) 10_557 10_557 ?
O4 Te1 Co1 133.73(8) . . ?
O4 Te1 Co2 46.27(8) . . ?
O4 Te1 Co2 46.27(8) 10_557 . ?
O4 Te1 Na1 121.05(8) 10_557 10_557 ?
O4 Te1 Na1 84.24(8) . 10_557 ?
O4 Te1 Na1 121.05(8) . . ?
O4 Te1 Na1 84.24(8) 10_557 . ?
O4 Te1 O4 88.05(15) . 10_557 ?
O4 Te1 Ba1 145.04(8) . . ?
O4 Te1 Ba1 91.87(8) 10_557 . ?
O1 Te1 Co1 91.099(10) . 10_557 ?
O1 Te1 Co1 91.099(10) . . ?
O1 Te1 Co2 76.14(11) . . ?
O1 Te1 Na1 146.85(7) . 10_557 ?
O1 Te1 Na1 146.85(7) . . ?
O1 Te1 O3 172.22(16) . . ?
O1 Te1 O4 91.53(11) . . ?
O1 Te1 O4 91.53(11) . 10_557 ?
O1 Te1 Ba1 53.52(8) . . ?
Te1 Co1 Na1 64.86(4) . . ?
Te1 Co1 Ba1 75.348(12) . . ?
Co1 Co1 Te1 178.876(10) 10_556 . ?
Co1 Co1 Na1 116.08(4) 10_556 . ?
Co1 Co1 Na1 92.13(5) 10_556 7_666 ?
Co1 Co1 Ba1 103.690(8) 10_556 . ?
Na1 Co1 Te1 87.81(5) 7_666 . ?
Na1 Co1 Na1 121.212(19) 7_666 . ?
Na1 Co1 Ba1 116.82(2) 7_666 . ?
O3 Co1 Te1 133.96(7) 7_666 . ?
O3 Co1 Co1 46.45(7) 7_666 10_556 ?
O3 Co1 Na1 50.66(9) 7_666 7_666 ?
O3 Co1 Na1 116.11(10) 7_666 . ?
O3 Co1 O2 90.41(12) 7_666 8_556 ?
O3 Co1 O4 95.09(9) 7_666 10_557 ?
O3 Co1 O4 74.49(11) 7_666 4_664 ?
O3 Co1 O1 93.47(10) 7_666 9_556 ?
O3 Co1 Ba1 136.30(9) 7_666 . ?
O2 Co1 Te1 89.29(7) 8_556 . ?
O2 Co1 Te1 37.88(7) . . ?
O2 Co1 Co1 89.66(7) 8_556 10_556 ?
O2 Co1 Co1 141.89(7) . 10_556 ?
O2 Co1 Na1 56.84(7) . . ?
O2 Co1 Na1 151.35(8) 8_556 . ?
O2 Co1 Na1 124.44(8) . 7_666 ?
O2 Co1 Na1 66.53(7) 8_556 7_666 ?
O2 Co1 O3 169.67(10) . 7_666 ?
O2 Co1 O2 95.33(12) . 8_556 ?
O2 Co1 O4 161.53(10) 8_556 4_664 ?
O2 Co1 O4 98.14(10) . 4_664 ?
O2 Co1 O4 76.95(9) . 10_557 ?
O2 Co1 O4 84.78(10) 8_556 10_557 ?
O2 Co1 O1 95.16(10) . 9_556 ?
O2 Co1 O1 89.51(12) 8_556 9_556 ?
O2 Co1 Ba1 53.16(7) 8_556 . ?
O2 Co1 Ba1 53.17(7) . . ?
O4 Co1 Te1 93.61(7) 4_664 . ?
O4 Co1 Te1 39.08(6) 10_557 . ?
O4 Co1 Co1 141.16(6) 10_557 10_556 ?
O4 Co1 Co1 87.51(7) 4_664 10_556 ?
O4 Co1 Na1 41.62(7) 4_664 . ?
O4 Co1 Na1 95.33(7) 4_664 7_666 ?
O4 Co1 Na1 82.36(7) 10_557 . ?
O4 Co1 Na1 50.57(8) 10_557 7_666 ?
O4 Co1 O4 86.03(10) 4_664 10_557 ?
O4 Co1 Ba1 103.37(7) 10_557 . ?
O4 Co1 Ba1 145.03(7) 4_664 . ?
O1 Co1 Te1 132.57(7) 9_556 . ?
O1 Co1 Co1 47.02(7) 9_556 10_556 ?
O1 Co1 Na1 133.95(9) 9_556 7_666 ?
O1 Co1 Na1 98.93(9) 9_556 . ?
O1 Co1 O4 169.74(11) 9_556 10_557 ?
O1 Co1 O4 101.74(12) 9_556 4_664 ?
O1 Co1 Ba1 66.43(9) 9_556 . ?
Ba1 Co1 Na1 105.486(19) . . ?
Te1 Co2 Te1 120.0 2_655 3_665 ?
Te1 Co2 Te1 120.0 2_655 . ?
Te1 Co2 Te1 120.0 3_665 . ?
Na1 Co2 Te1 90.0 4_665 . ?
Na1 Co2 Te1 90.0 4_665 3_665 ?
Na1 Co2 Te1 90.0 4_665 2_655 ?
Na1 Co2 Te1 90.0 7_666 2_655 ?
Na1 Co2 Te1 90.0 7_666 . ?
Na1 Co2 Te1 90.0 7_666 3_665 ?
Na1 Co2 Na1 180.0 7_666 4_665 ?
O4 Co2 Te1 103.02(7) 10_557 3_665 ?
O4 Co2 Te1 40.59(6) . . ?
O4 Co2 Te1 103.02(7) 11_657 . ?
O4 Co2 Te1 40.59(7) 3_665 3_665 ?
O4 Co2 Te1 103.02(7) 12_667 2_655 ?
O4 Co2 Te1 122.29(7) 3_665 . ?
O4 Co2 Te1 122.28(7) . 2_655 ?
O4 Co2 Te1 103.02(7) 3_665 2_655 ?
O4 Co2 Te1 122.28(7) 11_657 3_665 ?
O4 Co2 Te1 122.29(7) 12_667 . ?
O4 Co2 Te1 122.28(7) 2_655 3_665 ?
O4 Co2 Te1 122.28(7) 10_557 2_655 ?
O4 Co2 Te1 40.59(7) 12_667 3_665 ?
O4 Co2 Te1 103.02(7) 2_655 . ?
O4 Co2 Te1 40.59(6) 10_557 . ?
O4 Co2 Te1 40.59(6) 2_655 2_655 ?
O4 Co2 Te1 40.59(6) 11_657 2_655 ?
O4 Co2 Te1 103.02(7) . 3_665 ?
O4 Co2 Na1 51.27(7) 11_657 7_666 ?
O4 Co2 Na1 51.27(7) . 4_665 ?
O4 Co2 Na1 128.73(7) 2_655 7_666 ?
O4 Co2 Na1 51.27(7) 10_557 7_666 ?
O4 Co2 Na1 51.27(7) 2_655 4_665 ?
O4 Co2 Na1 51.27(7) 12_667 7_666 ?
O4 Co2 Na1 128.73(7) 12_667 4_665 ?
O4 Co2 Na1 128.73(7) 10_557 4_665 ?
O4 Co2 Na1 128.73(7) 11_657 4_665 ?
O4 Co2 Na1 128.73(7) 3_665 7_666 ?
O4 Co2 Na1 51.27(7) 3_665 4_665 ?
O4 Co2 Na1 128.73(7) . 7_666 ?
O4 Co2 O4 134.08(5) 11_657 3_665 ?
O4 Co2 O4 77.46(13) 3_665 12_667 ?
O4 Co2 O4 134.09(5) 11_657 . ?
O4 Co2 O4 85.00(10) 12_667 10_557 ?
O4 Co2 O4 85.00(10) 2_655 3_665 ?
O4 Co2 O4 85.00(10) 11_657 12_667 ?
O4 Co2 O4 85.00(10) 3_665 . ?
O4 Co2 O4 134.09(4) 12_667 . ?
O4 Co2 O4 85.00(10) 11_657 10_557 ?
O4 Co2 O4 77.46(13) 11_657 2_655 ?
O4 Co2 O4 134.09(5) 2_655 10_557 ?
O4 Co2 O4 85.00(10) 2_655 . ?
O4 Co2 O4 134.08(5) 2_655 12_667 ?
O4 Co2 O4 134.09(4) 3_665 10_557 ?
O4 Co2 O4 77.47(13) 10_557 . ?
Co1 Na1 Co1 119.863(6) 8_566 9_556 ?
Co2 Na1 Co1 92.13(5) 7_666 8_566 ?
Co2 Na1 Co1 92.13(5) 7_666 9_556 ?
O3 Na1 Co1 94.95(9) . 9_556 ?
O3 Na1 Co1 94.94(9) 3_565 8_566 ?
O3 Na1 Co1 123.66(10) . 8_566 ?
O3 Na1 Co1 123.66(10) 2_665 9_556 ?
O3 Na1 Co1 44.33(7) 3_565 9_556 ?
O3 Na1 Co1 44.33(7) 2_665 8_566 ?
O3 Na1 Co2 132.11(7) 3_565 7_666 ?
O3 Na1 Co2 132.11(7) . 7_666 ?
O3 Na1 Co2 132.11(7) 2_665 7_666 ?
O3 Na1 O3 79.95(11) 3_565 . ?
O3 Na1 O3 79.95(11) 2_665 . ?
O3 Na1 O3 79.95(11) 2_665 3_565 ?
O3 Na1 O2 68.89(10) . 2_665 ?
O3 Na1 O2 68.89(10) 2_665 3_565 ?
O3 Na1 O2 64.08(9) 3_565 3_565 ?
O3 Na1 O2 135.33(12) 2_665 . ?
O3 Na1 O2 135.33(12) . 3_565 ?
O3 Na1 O2 64.08(10) . . ?
O3 Na1 O2 64.08(9) 2_665 2_665 ?
O3 Na1 O2 135.33(12) 3_565 2_665 ?
O3 Na1 O2 68.89(10) 3_565 . ?
O3 Na1 O4 86.19(9) 3_565 6_554 ?
O3 Na1 O4 130.73(10) 3_565 5_564 ?
O3 Na1 O4 86.19(9) . 4_664 ?
O3 Na1 O4 130.73(10) 2_665 4_664 ?
O3 Na1 O4 143.42(10) 2_665 6_554 ?
O3 Na1 O4 130.73(10) . 6_554 ?
O3 Na1 O4 143.42(10) 3_565 4_664 ?
O3 Na1 O4 86.19(9) 2_665 5_564 ?
O3 Na1 O4 143.42(10) . 5_564 ?
O2 Na1 Co1 77.87(5) 3_565 9_556 ?
O2 Na1 Co1 42.03(5) 3_565 8_566 ?
O2 Na1 Co1 161.49(5) . 8_566 ?
O2 Na1 Co1 77.87(5) 2_665 8_566 ?
O2 Na1 Co1 42.03(5) . 9_556 ?
O2 Na1 Co1 161.49(5) 2_665 9_556 ?
O2 Na1 Co2 92.45(7) 3_565 7_666 ?
O2 Na1 Co2 92.45(7) 2_665 7_666 ?
O2 Na1 Co2 92.45(7) . 7_666 ?
O2 Na1 O2 119.819(11) 3_565 . ?
O2 Na1 O2 119.818(11) 3_565 2_665 ?
O2 Na1 O2 119.818(10) 2_665 . ?
O4 Na1 Co1 104.38(8) 6_554 8_566 ?
O4 Na1 Co1 47.06(6) 5_564 8_566 ?
O4 Na1 Co1 47.07(6) 6_554 9_556 ?
O4 Na1 Co1 120.66(9) 5_564 9_556 ?
O4 Na1 Co1 104.38(8) 4_664 9_556 ?
O4 Na1 Co1 120.66(9) 4_664 8_566 ?
O4 Na1 Co2 46.33(8) 4_664 7_666 ?
O4 Na1 Co2 46.33(8) 6_554 7_666 ?
O4 Na1 Co2 46.33(8) 5_564 7_666 ?
O4 Na1 O2 74.59(8) 4_664 . ?
O4 Na1 O2 138.45(12) 5_564 . ?
O4 Na1 O2 138.45(12) 6_554 2_665 ?
O4 Na1 O2 66.80(8) 6_554 . ?
O4 Na1 O2 74.59(8) 6_554 3_565 ?
O4 Na1 O2 66.80(8) 4_664 2_665 ?
O4 Na1 O2 74.59(8) 5_564 2_665 ?
O4 Na1 O2 66.79(8) 5_564 3_565 ?
O4 Na1 O2 138.45(12) 4_664 3_565 ?
O4 Na1 O4 77.57(12) 5_564 6_554 ?
O4 Na1 O4 77.57(12) 6_554 4_664 ?
O4 Na1 O4 77.57(12) 5_564 4_664 ?
Te1 O3 Co1 102.34(13) . 7_666 ?
Te1 O3 Co1 102.34(13) . 4_665 ?
Te1 O3 Na1 110.81(12) . . ?
Te1 O3 Na1 110.81(12) . 10_557 ?
Co1 O3 Co1 87.11(13) 4_665 7_666 ?
Co1 O3 Na1 146.84(17) 4_665 . ?
Co1 O3 Na1 85.01(6) 7_666 . ?
Co1 O3 Na1 85.01(6) 4_665 10_557 ?
Co1 O3 Na1 146.84(17) 7_666 10_557 ?
Na1 O3 Na1 84.22(15) . 10_557 ?
Te1 O2 Co1 100.27(11) . . ?
Te1 O2 Co1 129.22(13) . 9_556 ?
Te1 O2 Na1 91.45(10) . . ?
Te1 O2 Ba1 116.26(11) . . ?
Co1 O2 Co1 124.64(12) . 9_556 ?
Co1 O2 Na1 71.44(7) 9_556 . ?
Co1 O2 Na1 86.08(9) . . ?
Co1 O2 Ba1 89.52(8) . . ?
Co1 O2 Ba1 88.95(8) 9_556 . ?
Ba1 O2 Na1 152.28(10) . . ?
Te1 O4 Co1 100.27(11) . 4_665 ?
Te1 O4 Co1 95.21(10) . 10_557 ?
Te1 O4 Co2 93.14(10) . . ?
Te1 O4 Na1 159.05(14) . 4_665 ?
Co1 O4 Co1 93.98(10) 4_665 10_557 ?
Co1 O4 Co2 105.01(11) 4_665 . ?
Co1 O4 Na1 100.66(10) 4_665 4_665 ?
Co1 O4 Na1 82.36(10) 10_557 4_665 ?
Co2 O4 Co1 157.53(13) . 10_557 ?
Co2 O4 Na1 82.40(9) . 4_665 ?
Te1 O1 Co1 124.74(12) . 8_556 ?
Te1 O1 Co1 124.74(12) . 5 ?
Te1 O1 Ba1 97.81(10) . 4 ?
Te1 O1 Ba1 97.81(10) . . ?
Co1 O1 Co1 85.96(13) 8_556 5 ?
Co1 O1 Ba1 76.69(6) 8_556 . ?
Co1 O1 Ba1 136.13(14) 8_556 4 ?
Co1 O1 Ba1 76.69(6) 5 4 ?
Co1 O1 Ba1 136.13(15) 5 . ?
Ba1 O1 Ba1 88.47(9) . 4 ?
O2 Ba1 O2 68.61(5) 7_556 2 ?
O2 Ba1 O2 180.0 8_556 2 ?
O2 Ba1 O2 68.61(5) . 9_556 ?
O2 Ba1 O2 68.61(5) 7_556 3 ?
O2 Ba1 O2 111.39(5) . 3 ?
O2 Ba1 O2 111.39(5) 2 3 ?
O2 Ba1 O2 180.0 7_556 . ?
O2 Ba1 O2 68.61(5) 8_556 . ?
O2 Ba1 O2 68.61(5) 8_556 3 ?
O2 Ba1 O2 68.61(5) 2 9_556 ?
O2 Ba1 O2 111.39(5) 2 . ?
O2 Ba1 O2 111.39(5) 7_556 9_556 ?
O2 Ba1 O2 111.39(5) 8_556 9_556 ?
O2 Ba1 O2 111.39(5) 7_556 8_556 ?
O2 Ba1 O2 180.0 9_556 3 ?
O2 Ba1 O1 59.00(8) . 2 ?
O2 Ba1 O1 118.21(7) 7_556 9_556 ?
O2 Ba1 O1 54.13(8) 2 2 ?
O2 Ba1 O1 61.79(7) 8_556 . ?
O2 Ba1 O1 118.21(7) 2 . ?
O2 Ba1 O1 54.13(8) 9_556 9_556 ?
O2 Ba1 O1 125.87(8) 9_556 3 ?
O2 Ba1 O1 54.13(8) 3 3 ?
O2 Ba1 O1 59.00(8) 8_556 9_556 ?
O2 Ba1 O1 121.00(8) 2 9_556 ?
O2 Ba1 O1 125.87(8) 3 9_556 ?
O2 Ba1 O1 61.79(7) . 9_556 ?
O2 Ba1 O1 118.21(7) . 3 ?
O2 Ba1 O1 118.21(7) 3 2 ?
O2 Ba1 O1 61.79(7) 9_556 2 ?
O2 Ba1 O1 61.79(7) 3 8_556 ?
O2 Ba1 O1 125.87(8) 7_556 . ?
O2 Ba1 O1 59.00(8) 3 . ?
O2 Ba1 O1 59.00(8) 9_556 7_556 ?
O2 Ba1 O1 125.87(8) 8_556 2 ?
O2 Ba1 O1 121.00(8) 3 7_556 ?
O2 Ba1 O1 121.00(8) 7_556 2 ?
O2 Ba1 O1 59.00(8) 7_556 8_556 ?
O2 Ba1 O1 61.79(7) 7_556 3 ?
O2 Ba1 O1 54.13(8) 8_556 8_556 ?
O2 Ba1 O1 121.00(8) 8_556 3 ?
O2 Ba1 O1 125.87(8) 2 8_556 ?
O2 Ba1 O1 54.13(8) 7_556 7_556 ?
O2 Ba1 O1 121.00(8) . 8_556 ?
O2 Ba1 O1 54.13(8) . . ?
O2 Ba1 O1 118.21(7) 8_556 7_556 ?
O2 Ba1 O1 121.00(8) 9_556 . ?
O2 Ba1 O1 61.79(7) 2 7_556 ?
O2 Ba1 O1 118.21(7) 9_556 8_556 ?
O2 Ba1 O1 125.87(8) . 7_556 ?
O2 Ba1 O1 59.00(8) 2 3 ?
O1 Ba1 O1 76.70(7) 7_556 9_556 ?
O1 Ba1 O1 103.30(7) 7_556 3 ?
O1 Ba1 O1 103.30(7) 8_556 . ?
O1 Ba1 O1 76.70(7) 2 . ?
O1 Ba1 O1 103.30(7) 2 9_556 ?
O1 Ba1 O1 180.0 8_556 2 ?
O1 Ba1 O1 76.70(7) 8_556 9_556 ?
O1 Ba1 O1 180.0 7_556 . ?
O1 Ba1 O1 103.30(7) 8_556 3 ?
O1 Ba1 O1 103.30(7) 7_556 2 ?
O1 Ba1 O1 76.70(7) 2 3 ?
O1 Ba1 O1 76.70(7) . 3 ?
O1 Ba1 O1 180.00(13) 9_556 3 ?
O1 Ba1 O1 103.30(7) . 9_556 ?
O1 Ba1 O1 76.70(7) 7_556 8_556 ?

_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details 
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
- Detector area scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.541
_oxdiff_exptl_absorpt_empirical_full_min 0.659
_exptl_crystal_recrystallization_method 'From the Melt'
_exptl_crystal_preparation       'Magnetic properties'
